* Your assessment is very important for improving the workof artificial intelligence, which forms the content of this project
Download Prediction of stress-strain relationships in low
Document related concepts
Retrospective Theses and Dissertations 1960 Prediction of stress-strain relationships in lowcarbon steel Wilbur Barrett Ratterree Iowa State University Follow this and additional works at: http://lib.dr.iastate.edu/rtd Part of the Applied Mechanics Commons Recommended Citation Ratterree, Wilbur Barrett, "Prediction of stress-strain relationships in low-carbon steel " (1960). Retrospective Theses and Dissertations. Paper 2627. This Dissertation is brought to you for free and open access by Digital Repository @ Iowa State University. It has been accepted for inclusion in Retrospective Theses and Dissertations by an authorized administrator of Digital Repository @ Iowa State University. For more information, please contact [email protected] PREDICTION OF STRESS-STRAIN RELATIONSHIPS IN LOW-CARBON STEEL by Wilbur Barrett Ratterree A Dissertation Submitted to the Graduate Faculty in Partial Fulfillment of The Requirements for the Degree of DOCTOR OF PHILOSOPHY Major Subject: Theoretical and Applied Mechanics Approved: Signature was redacted for privacy. In Work Signature was redacted for privacy. tment Signature was redacted for privacy. Des... — Jollege Iowa State University of Science and Technology Ames, Iowa I960 ii TABLE OF CONTENTS Page INTRODUCTION 1 SURVEY OF LITERATURE 4 ANALYSIS 44 EXPERIMENTAL PROCEDURE 60 CALCULATIONS AND RESULTS 65 CONCLUSIONS 86 RECOMMENDATIONS FOR FUTURE WORK 88 SYMBOLS EMPLOYED 89 LITERATURE CITED 91 ACKNOWLEDGMENTS 95 1 INTRODUCTION Although the different metals may vary in color, strength, ductility, electrical conductivity, thermal conductivity and density, and even though these and other properties may vary in different directions, each of the metals has a crystalline structure. In one or more planes through the crystals, planes of maximum atomic density, shear will occur more easily than in other planes. planes. These are known as planes of weakness or slip It is possible under careful control to grow single crystals of appreciable size, but the metals available for in dustrial use are manufactured under such conditions that they are composed of millions of crystals. These many small crys tals, even though each is regular in its atomic formation, solidify from the melt with their planes of weakness in all possible directions; hence, all commercial metals, e.g. lowcarbon steel, are characterized by extreme randomness of crys tal orientation. A single crystal has different strengths in different directions; e.g. if the direction of loading is parallel to a slip plane slip will occur at a lower magnitude of load than if the direction is perpendicular to the slip plane. The random orientation of the crystals in a specimen allows some of the crystals to be in a more favorable position to resist loads than other crystals. Therefore, when a specimen is subjected to tension, some of the crystals begin to slip before the rest 2 do and twinning frequently occurs. As the tension increases, more of the crystals will slip and some of them will also undergo a partial rotation. The deformation that occurs before slip or rotation occur is an elastic deformation, and the specimen will recover its shape if unloaded; that deformation occurring as the result of slip or rotation is permanent and is termed plastic strain. It follows, therefore, that the axial strain which develops as axial stress is applied may in clude both elastic and plastic strain. Some of the properties of metals are sensitive to the internal structure of the metals while others are not; these structure sensitive properties include mechanical strength, elasticity, hysteresis and ductility (1). These properties are changed by work-hardening, which is the result of straining part of the metal into the plastic range. In engineering practice these and other properties are found and presented with the aid of a conventional stress-strain diagram which is plotted from data obtained in an axial loading test. Most metals obey Hooke's law, at least approximately, over a limited range. When this range is exceeded the change in the structure sensi tive properties becomes much more pronounced, and in the case of low-carbon steel an avalanche of slip occurs producing the conventional yielding phenomenon. If the steel is cold worked sufficiently the yielding is not so catastrophic, if it occurs at all, but the structure sensitive properties still undergo a 3 marked change. One of the properties which is extremely sensitive to changes in the treatment of the metal is the damping capacity (2), which is frequently determined from the hysteresis. Therefore, any treatment which affects the other structure sensitive properties should be reflected also in a change in the damping capacity. It is known that damping is a function of stress (3-4), although the precise function may not be known; it is also known that strain is a function of stress. Therefore, a correlation should exist between damping and strain, and we should be able to predict stress-strain relations from corresponding stress-damping relations. The purpose of this investigation is to make such a prediction. 4 SURVEY OF LITERATURE The characteristic of matter which today is designated damping has at various times been termed internal friction, molecular friction, elastic hysteresis, and crackless plastic ity by different investigators (2). Lord Kelvin (5), a pioneer in this area, described it as a molecular friction which he called the viscosity of solids. He observed in 1864 that the rate of subsidence of vibration in matter was greater after oscillating for a time than it was at the beginning of oscillation. For his work he used a wire as a torsional pendu lum. He further observed that when the tension in the wire was increased, the viscosity was also greatly increased at first; but that day after day this solid viscosity decreased until it was no greater than it was without the increased tension. Also the subsidence over a given amplitude range was increased if the initial amplitude was increased. In a wire vibrated most of each day for several days, the molecular friction was greater than it was for a similar wire kept quiescent except during each experiment. The dying out of the vibration is not due to resistance which is linearly proportional to the veloc ity of the vibration; but appears to be due, at least partially, to imperfect elasticity, i.e. "elastische Nachwirking." As Thompson (2) remarked, interest in and investigation of damping was rather sporadic until about three decades ago. 5 The revival of interest was due primarily to the increasing operating speeds of modern machinery with resulting critical vibration. The attempt to determine which materials are most efficacious in damping vibrations prompted a continued interest in this characteristic. For instance, there are conditions under which a crankshaft made of cast iron is preferable, as far as service life is concerned, to the same part made of steel since the damping capacity of cast iron is much greater than that of steel. The metals used in machines and structures are polycrystalline materials with the axes of the crystals randomly oriented. The very randomness of orientation, while tending to impart overall isotropy to the metal, makes the determina tion of precise, fundamental relations difficult to obtain. For this reason a great deal of the investigation of damping has been done on single crystals, and frequently at stresses below the accepted proportional limit. According to Joffe (6), elastic after-effect, elastic hysteresis, and elastic fatigue do not occur in single, pure, regularly built crystals. These phenomena are the results of such things as the irregularities in heterogeneous material, stress in excess of the elastic limit and subsequent rupture in small weak regions within the material, and the interaction between crystalline grains. Accurate measurements show that Hooke's law does not hold 6 to the elastic limit, and that the nominal proportional limit decreases with increasing accuracy of measurement. From this Joffe concluded there is no true proportional limit. This can be interpreted to mean that even at low stress levels a small amount of plastic deformation occurs which leads to his obser vation that the elastic limit is reached upon the occurrence of small elementary glidings between crystal grains or inside the crystal itself. The effect of these glidings can be ob served on polished surfaces and are Lueders1 lines. At higher stresses this gliding or sliding is accompanied by a rotation of and within the crystals and a breaking up of the crystals into many parts, although transparency in the case of rock salt is not destroyed. From this Joffé concluded that crystals have a property which he termed the destruction limit, which is observed in Laue x-ray pictures by the single spots changing to radial beams. At 500 C no change in the x-ray picture of rock salt could be seen after 24 hours at a load 2 percent below this destructive limit, while if the load is 2 percent above the limit a change is observed in a single second. He stated that the phenomenon depends on internal stresses and temper ature but is independent of crystal size, and that the limit is the same for tension or compression. Rock salt from different localities, with different impurities and different surface treatments gave destruction limits within 2 percent 7 of each other. Joffe's experiments revealed that if only gliding of planes of atoms within the crystal occur the x-ray pattern is not changed. A permanent set due to gliding which appears before the x-ray pattern changes may be removed by stress of opposite sign. However, the set which occurs at the destruc tion limit is irreversible. Although the x-ray pattern changes at the destruction limit transparency does not change, and cohesion increases despite the breakdown of the larger crystal into small crystalline fragments. He concluded that in plastic flow separation does not exceed atomic distances. Joffe enunciated two limits: first, the elastic limit is the stress at which the first permanent set due to slip with negligible rotation appears; second, the destruction limit is the stress at which crystal fragmentation and rotation occur which is indicated by a change in the x-ray pattern. This is accompanied by interstitial residual stress which can be re moved by annealing. The grains become smaller due to fragmentation, but the crystal lattice remains the same. In a study on the endurance of constructional materials Becker and Foppl (7) pointed out that the usual assumption in strength of materials of solids being elastic is not true. They referred to fatigue failures of machine parts at stresses below the usual proportional limit as examples of the failure of the assumption. They also pointed out that vibration or 8 stress changes produce structural changes in the materialmost of their paper deals with polycrystalline steel—which are determined by static test. Plastic deformation occurs below the usual elastic limit although it is much less than the elastic strain. But they maintained that these plastic strains exert an essential influence on the continued use of the material. An example is cited in which at the elastic limit the nominal elastic strain was 0.10 percent of which 3 percent was plastic deformation. They believed that torsion tests are best for determining fatigue characteristics. They claimed the existence of an endurance deformation corresponding to the endurance limit; however, this deformation does not obey Hooke's law since the vibration strength is greater than the proportional limit as determined by static tests. (This implies dynamic strength characteristics greater than static strength values.) Their experience indicates that damping is independent of frequency up to 2600 cpm. They also claimed that the damping capacity can be determined from a static test; their method of doing this was to take the ratio of the hysteresis to the total energy absorbed in cycles of slow loading and unloading as the damping capacity. It should be pointed out that they have implied different characteristics in dynamic and static loading. It should be remarked that most of the properties of 9 materials used by design engineers are determined from static or essentially static tests. Only in recent years has there been much continued effort toward determining properties present in or controlling dynamic situations. Even today, there are no standard clear-cut methods for obtaining dynamic characteristics. In fact, most of the effort in the past has been in improving and verifying procedures for obtaining values from static tests, which are—with or without modifi cation—used for dynamic design. In 1929, Templin (8) presented an interesting paper on the proportional limit which is the limiting stress at which unit stress is proportional to unit strain. While conceding the proportional limit may be a safe limit for the application of the usual mathematics and mechanics in the design of metal structures, he pointed out many difficulties are involved in its determination, and to use it as a routine specification causes unwarranted hardships to manufacturers. The material tested, the test specimen used, the testing apparatus used, the testing procedure followed, and the inter pretation of the results obtained are factors affecting the value of the proportional limit. Not only are metals as used and tested generally heterogeneous, anisotropic crystalline materials; but they also vary in performance due to voids, inclusions, seams, grain sizes, segregations, and non-uniform tempers. Any of these factors may cause local yielding or 10 failure with the result that an excessive amount of testing is required to get reliable values. Variation in strain, straightness, and dimensions of the specimen give scattered values for the proportional limit while affecting the ultimate stress or yield strength at a specified offset but slightly. Machining test specimens to size may either induce or relieve residual stress and strain. The lower the speed of testing, i.e. a decrease in the rate of deformation, the lower will be the proportional limit. The scale used in plotting unit strain in the stress-strain curve greatly influences the pro portional limit, while the yield strength and ultimate stress remain the same. His conclusion was that when the factors affecting the proportional limit can be rigorously controlled the results have value in defining the limit to which Hooke's law may be validly applied in design; however, since yield strength has significantly less variation in range of values the latter is a better specification. In discussing Tempiin's paper, Moore (9) stated that yield strength marks the beginning of inelastic action by a rather crude method, while proportional limit does the same thing using a fairly delicate method. McVetty (10) stated that "Proportional limit, if rigorously applied, refers to a stress which cannot be measured by any means now known and which marks the so-called limit of a proportionality which does not exist." However, he continued, if allowance is made 11 for uncontrollable variables and suitable precautions are exercised, the apparent proportional limit is extremely valuable, particularly at elevated temperatures and in re search investigations. Withey (11) felt that the most important information given by the proportional limit or the yield point is the intensity of stress which the material can resist without significant plastic deformation. Tuckerman (12, p. 538) felt a "twinge of conscience" each time he reported a proportional limit because, strictly speaking, "it is not a characteristic of the material but a hazy composite of material properties, testing technique, method of plotting, and personal equation." To arrive at a more reliable value he plotted the experimental stress-strain data and drew in the best straight line which he then used to calculate strain. He next plotted stress against actual strain minus calculated strain to assist in determining the proportional limit. Several illustrations are given in his discussion. Brophy (13) attempted to correlate some of the mechanical properties of materials with the ability of the material to damp out free vibration. He used the designation damping capacity for this property and defined it as the decrease in amplitude per cycle divided by the original amplitude at various stress levels of a free vibration. For his work he used a Fôppl-Pertz torsional vibration machine. It is shown in his paper that damping capacity varies with stress, but 12 that for iron and steel there is a measurable value at very low stresses. Consequently, since the vibration damping is due to plastic deformation, there is considerable plastic action even at the lowest stresses which leads to the conclu sion that no true elastic limit exists. The smaller the damping capacity is the nearer is a material to being per fectly elastic. Cold work influences the magnitude of the damping capacity, and increasing the temperature below the strain hardening temperature limit increases the damping capacity. Brophy claimed a general correlation exists between damping and creep, but he has not confirmed a general decrease of damping with annealing. From a later paper (14) dealing with the influence of grain size on damping capacity, and the use of damping capacity as a measure of the damage to steel resulting from fatigue due to overstress and notches, one draws the following conclusions: (a) increasing the grain size of a metal increases its damping capacity; (b) in any cycle of stress during free vibration both elastic and plastic deforma tion are present, but the decrease in amplitude represents plastic action only; (c) high damping capacity is associated with high resistance to notch fatigue; and (d) high damping is associated with low resistance to alternating overstress. Foppl (15) stated that all ferrous metals used in con struction can withstand a certain amount of plastic, as well as elastic, distortion for an indefinite number of stress 13 cycles without risk of ultimate failure. The damping capacity, (// , may be defined as the ratio between the area of the hysteresis loop and the strain energy stored in the specimen when it is in the extreme position under cyclic stressing. He indicated that it may also be represented by the ratio, X , between the plastic strain and the total strain, which at low plastic strains is approximately the ratio between plastic and elastic strain. He stated X is approximately 0.2^ . The accompanying stress-strain diagram, Fig. 1, illustrates this. retical elastic cycling. Straight line A represents theo B represents actual cycling. Area of loop B represents hysteresis. Diagonally crosshatched triangular areas represent maximum strain energy absorbed per cycle. Even with large plastic strains, e.g. = 0.1€ e^, many steels go through millions of cycles without deterioration. Tests designed to show a definite and limited capacity to dissipate energy by internal friction have yielded negative results. At least for steel, if the stress is not excessive, the capacity for dissipating energy in the form of heat is unlimited. Foppl tested one specimen at 700 cpm with <// = 0.5 for each cycle, thereby dissipating enough energy as heat to maintain the specimen at 100 C above room temperature for three years without any signs of damage appearing. Damping capacity is a property of the material which is 14 -> Fig. 1. Hysteresis loop—from Foppl (15) 15 dependent on maximum strain amplitude, specimen temperature and the number of cycles completed. Damping is no indication of impending fatigue failure, according to Foppl, nor does it change in the sense of becoming exhausted in the course of time. At any point in a specimen for an elementary cube there exists a certain stress, a certain strain, and a certain damp ing capacity. The point of failure of a specimen in static tension depends on a weak spot in the material--ultimate stress is not a mean value but a least favorable value— whereas damping capacity is a mean value and does not depend on a weak spot; i.e. every element of the specimen contributes a definite amount to the total damping. If the fatigue limit is not exceeded at any point by cyclic stress there are only two independent quantities— <T, stress and 6, strain—to be found for any particle or element. These experimental measurements may be represented by either of the curves CT= f (<£= ) or = f'(6 ) = E . For small 6, E = EQ which is Young's modulus. small, E = EQ - AE. If € is not AE is due to the plastic strain in the material. Foppl stated that v-è4£. and if <ÛE «< E, then C » 0.2. He agreed with others that the damping is due to the plastic strain, and if the latter is 16 increased the former will also increase. He cautioned that the ends of the specimen must be tightly gripped to prevent damping occurring at the grips rather than in the specimen. Nadai (16) stated that although the stress at which plastic yield occurs in polycrystalline metals depends on the plastic strain and the time rate of change of plastic strain, for soft metals at low temperatures one can validly assume the plastic yield depends only on the permanent strains. (He did not give a temperature range, and whether the temperature is high or low was apparently its value relative to the melting point.) The low range of temperatures is characterized by the metal strain-hardening, while the upper or elevated range is characterized by the metal creeping. He stated that plastic action does not seem to depend on the mean octahedral normal stress, and that strain-hardening depends on the "natural" or true shearing strain. Having plotted conventional tensile stress-strain and true stress-strain diagrams from experimental data, he then constructed predicted conventional stress-strain diagrams for various amounts of cold working (i.e. prestretch ing). Spath (17) remarked that there are differences of opinion as to the existence of a damping limit and as to the use of damping techniques for testing procedures. Among other things damping depends on the tension in the specimen. There do not seem to be any apparent relationships between static and 17 dynamic tensile strength values; perhaps, in his opinion, damping tests will prove to be the connecting link between static and dynamic testing. When changes occur in the value of damping it is an indication that changes have occurred in the material which will produce changes in characteristic static strength values. He believed a close relationship exists between damping, proportional limit, yield point, etc., but that a "shakedown"--specimen subjected to many cycles of stress before testing--must be run in order to obtain repre sentative reproducible values of damping capacity. In an attempt to learn what occurs during the transition from the elastic to plastic state, Winlock and Leiter (18) noted that in deep drawing of light-gage steel surface depres sions occur under tension and surface elevations occur under compression. These deformations are due to highly localized plastic flow and are known as Lueders1 lines or "stretcher strains." Many metals, e.g. aluminum, do not show an abrupt change in their stress-strain diagrams when the metal changes from essentially elastic to non-elastic action; the deformation in the plastic range in such cases is described as uniform and not localized. On the other hand, low carbon steel without previous cold work acts elastically to the upper yield point, A, at which stress plastic action occurs at a localized point in the specimen, as illustrated in Fig. 2. The resistance of the 18 /W 6 Fig. 2. Tensile stress-strain diagram—from Winlock and Leiter (18) 19 specimen to further deformation as registered on a universal type testing machine then drops to L, the lower yield point, as the metal adjacent to the first point becomes plastic. Winlock and Leiter (18, p. 562) stated that "The elongation required to produce complete plastic deformation varies with the speed of deformation, but under ordinary conditions is some 5 percent." It should be emphasized that when substantial plastic action begins, it is no longer necessary to have present the load which the metal resisted elastically (point A) to have plastic action continue. If the steel has undergone previous cold work of sufficient magnitude the abrupt change will not appear and the curve will be smooth such as OYLM. They claimed that mathematical equations de scribing the region A-L of the diagram cannot be established on the basis of homogeneous or heterogeneous flow since neither uniform nor non-uniform plastic flow occurs. If the steel were to act as most other metals, then plastic action might be expected to occur at the stress Y, the extrapolation of M-L back to the elastic range. For some un explained reason steel, however, in the annealed condition overshoots Y and continues to act elastically up to A. At this stress it yields locally, and since it can now exert only resistance Y it deforms rapidly along A-a. At the next instant the adjacent elements deform plastically at stress B along B-b an amount equal to B-b. This continues for more and 20 more metal as indicated by C-c until apparently all of the metal undergoes plastic action. The load on the specimen as registered by the testing machine drops for the following reasons: first, the resistance to further plastic action is only Y; second, there is stress concentration at the ends of the first and subsequent local constrictions; third, there is now present an increasing amount of cold-worked, i.e. plasti cally deformed, metal; and fourth, the speed of deformation of the increments as they become plastic is greater than the speed of the testing machine head. The registered load does not drop to Y but only to L, the lower yield point, because a balance is attained between the increase in resistance due to further plastic deformation, the increase in resistance due to the high speed of deformation, and the presence of metal in other parts of the gage length which must be stressed elasti cally to A before plastic action occurs. Uniform elongation, after plastic action sets in, does not begin at the end of the yield point range, according to Winlock and Leiter; instead, it begins when all parts of the specimen have undergone deformation equal to that attained by the first increment which deforms plastically. Since the on set of plastic action is highly localized, there exists during yielding regions of both elastically and plastically deformed metal. Work-strengthening is caused by plastic deformation. So 21 long as both plastic and elastic regions are present, the be havior of the metal under plastic action is obscured. The rate of work-strengthening is the rate of increase of only that stress required to cause further plastic action in metal which has already been plastically deformed. If the steel is sufficiently cold-worked before testing, the upper yield point disappears, and the stress-strain curve is like OYLM with sub stantial plastic action occurring at stresses below A. Contractor and Thompson (19) in reporting investigation of the damping capacity of steel stated that damping is present at stresses as low as 200 psi and that very likely it is present at zero stress. (This means that hysteresis occurs even at low so-called elastic stress.) They agreed with the previous findings that plastic deformation increases damping capacity and that the specimen must be held firmly in the grips or energy loss occurs there giving unduly high damping capacities. They found that, in general, damping capacity increases with load. Hatfield et al. (20a, p. 273) defined damping as "the operation of influences which by resisting the motion and ab sorbing energy from the system, restrict and tend to stop the vibration." Solid friction or damping is not of a viscous nature, i.e. it is not proportional to velocity, but is "nearly independent of speed" except at extreme speeds. Their view was that solid damping is due to "imperfections in the 22 elastic properties" of the materials. In a number of tests on various materials, including mild steel, they found that damp ing increases with load within the usual elastic range—no data beyond the proportional limit is reported--and that the reaction of damping to temperature changes varies with the metal. Mild steel increases in damping up to 100 C, then re cedes to 300 C, after which it again increases. Between 460 C and 500 C a relatively abrupt increase in damping occurs in mild steel, e.g. from 3.45 to 5.60 percent per cycle. Slight differences in heat treatment which produce significant changes in mechanical properties also cause significant changes in damping capacity. These three investigators found austenitic steels give relatively low values of damping, mild steels give intermediate values, and some stainless steels give very high values. They also stated that attempts to relate damping characteristics with proportional limit values have shown poor correlation. Their work was performed with a modification of the torsional damping recorder manufactured by the Cambridge Instrument Company. Low and Garofalo (20b) considered the proposed analytical expression, 6" = K<^n, relating true stress to true strain in the plastic region. In this expression is the load divided by the instantaneous area, K and n are material constants, and & is true unit strain. If (fQ is the nominal stress, and 6 is the nominal strain, then û" = (fQ (1 + € ); however, in the 23 true strain, S- ln(l + ex ), £x is the plastic unit strain €x - € - only which is obtained from the difference between . They stated that e and 6' is usually not significant for e greater than 5 percent. Their tests on seven different steels and two aluminums indicated that the proposed expres sion is generally valid, the only exception in their tests having been austenitic steel. They believed a phase change in the austenitic steel occurred during the test and caused a deviation from the prediction. They also noted that the rela tion is not valid in the immediate region of discontinuous yielding for mild steel which shows a marked yield point, but that it is valid elsewhere. K and n are determined from a logarithmic plot of the experimental data. Zener 121), as well as Spath (17) and Becker and Foppl (7) stated that in periodic oscillation strain lags stress for actual metals by some angle which is a measure of internal friction or damping. elastic materials. This angle would be zero for truly Zener proposed equations relating functions for creep, stress, dynamic modulus, and internal friction. He maintained that plastic deformation of all crystalline materials occurs in isolated regions called slip bands rather than homogeneously throughout the metal. In addition he maintained that the slip bands act as isolated viscous regions, giving rise to anelastic behavior. This viscous nature of the slip bands, said Zener, renders the yield stress two or three orders of magnitudes less than theoretical 24 i.e. less than e^E 7 o where e„, o7 the elastic strain at fracture, is approximately 0.10. The formation of slip bands is a cata clysmic process and starts at a stress which, theoretically, is inversely proportional to the grain size. He claimed internal friction is a single valued function of stress ampli tude, and that in the vicinity of room temperature the internal friction due to plastic deformation is independent of frequency. According to Zener anelasticity is the property of solids by virtue of which stress and strain are not single valued functions of each other in the low stress range in which no permanent set occurs. He thought of internal friction as the capacity of solids to convert vibrational energy into internal energy. Thompson (2, p. 1) defined damping capacity as "that property of a solid in virtue of which it can, of itself, dissipate internal vibrations, and hence prevent their attain ing dangerous dimensions." He stated there was unanimity of opinion that damping capacity of metals is an extremely sensitive property which is greatly affected by very small changes in the treatment of metal. To almost all other state ments flatly contradictory opinions can be found. He claimed that enough data exist in the literature "to make it reasonably certain that none of the normal mechanical tests provide any criterion from which the damping properties can be predicted." He suggested the existence of a relationship between damping 25 capacity and fatigue limit which is analogous to that between static ductility and tensile strength. The sensitivity of damping to small changes in treatment shows that this property is something which exerts a much smaller and sometimes negli gible effect on ordinary static tests. Hanstock (22) compared thermal vibration due to fluctu ating temperature and mechanical vibration due to fluctuating loads or free vibration resulting from a change in load. He gave the scheme shown in Fig. 3 for the dissipation of mechanical vibrational energy. He observed that damping effect is characteristic of the metal and its metallurgical state and arises from some process or processes occurring in the metal. Also, the stresses due to oscillation are proportional to the amplitude of oscilla tion, and, for small stresses, the damping is relatively insensitive to amplitude. In discussing several methods of measuring damping, he pointed out the advantages and disad vantages of using a fine wire as an oscillating torsional pendulum. The advantages are (a) the method has simplicity, (b) the pendulum can be operated readily in an evacuated chamber, (c) the temperature can be easily controlled; the disadvantages are (a) the wire is thin and may not represent metallurgically the material in general, (b) it is difficult to grip ends firmly enough to prevent energy losses at the ends, (c) only low torsional stresses are imposed. Vibrational conduction losses. Sound waves Disturb atom arrangement Friction at faults and cracks Vibration energy Viscous and plastic effects Rearrange atoms Magnetic effects Thermal vibration Irise of temperature) Thermal radiation, conduction, convection Fig. 3. A diagram for the dissipation of mechanical vibrational energy--from Hanstock (22) 27 At the same order of stress as the static proportional limit there is a marked increase of damping with increase of stress. This increase in damping is due mainly to plastic action, and since the metal properties may change under such action there is an interrelation between stress, duration of vibration, and damping. At stresses below the proportional limit, the damping is nearly constant and depends but little on plastic action; hence, it is concluded that metal is not altered much below the proportional limit. Hanstock observed that damping increases with temperature for non-magnetic metals, and past the magnetic transformation temperature the phenomenon is in evidence for magnetic metals too. He has shown an exponential relation between stress and damping for aluminum alloys under short time vibrations. This relation is governed by the proportional limit, the tensile strength, stress concentration due to submicroscopic lattice faults, and a factor expressing the strain in the lattice necessary to cause one atom to slip past another. Long time vibrations first raise and then lower the proportional limit much as annealing lowers the proportional limit. It is common knowledge that the presences of imperfections in metals weaken them tremendously. An excellent qualitative discussion of one type of imperfection, a dislocation—proposed independently by G. I. Taylor and E. Orowan in 1934—, was given by Cuff and Schetky (23). They discussed an edge 28 dislocation and a screw dislocation. an orderly array of many atoms. A crystal is composed of If the atoms are in register except at a region in the crystal where there is one more row of atoms on one side of the region than on the other, this region is known as an edge dislocation. AB in Fig. 4 is the line of the edge dislocation, which is a region of small finite cross section running through the crystal. The lattice is compressed on the side of the extra row of atoms and extended on the other side. This region is then of higher energy than the rest of the crystal an.\ since energy tends toward a minimum for equilibrium, the region acts like a stretched elastic band. This means the dislocation line resists being bent or curved. The line of an edge dislocation is perpendicular to the slip direction. The force required to move a dislocation through the crystal is less than the force required to make an entire plane of atoms slip. Dislocations of like sign repel and of unlike sign attract each other. When a dislocation line is blocked by some other type of im perfection or grain boundary, other dislocations pile up behind it like "automobiles at a red light"; the motion cannot resume until the anchored dislocation can be torn free, thus producing strain hardening and strengthening. If dislocations interact, thereby removing the dislocation, the path of easy slip is removed and thus the material is strengthened. If slip occurs parallel to the dislocation line, as 29 Fig. 4. Edge dislocation—from Cuff and Schetky (23) 30 happens when only one end of a dislocation is anchored, a screw dislocation is produced. Under continued stressing the dislocation pivots about the anchored end and produces an atomic displacement perpendicular to the dislocation line for each revolution. Thus such a dislocation is never used up. Cuff and Schetky claimed that--at the time of their paper, 1955--the actual behavior of the numerous interacting disloca tions in a real metal could not be predicted. Woolley (24) explained work-hardening on the basis of either exhaustion theory or the hardening theory. At grain boundaries or other places of lattice misfit there exists a distribution of high stress regions called partial disloca tions. When the minimum stress necessary to liberate these dislocations is applied, i.e. the activation stress, they become mobile and travel through the crystal until they en counter some barrier. After encountering the obstacle a dislocation contributes but little more, or no more, to plastic flow, and hence the distribution becomes exhausted. The extension under tension is the result of the aggregate dislocation motion. The number of dislocations is approximate ly proportional to the rate of change of strain with stress. The hardening theory assumes that each of the dislocations has approximately the same activation stress, the elastic limit. When this stress is exceeded plastic flow occurs, the activa tion stress is raised, and increased stress must be applied to 31 produce further plastic flow. Woolley said the rate of change of strain with stress has no physical meaning in the hardening theory. In either theory if the specimen is loaded past the activation stress, unloaded and reloaded, the reloading action is elastic until the previous maximum stress is reached when plastic action resumes. Dislocation motion is associated only with plastic action. Only relatively few of the dislocations are undirectional; i.e. if the stress is reversed most of the previously blocked dislocations contribute nothing more to the plastic action. In attempting to explain the plastic properties of a crystal, Cottrell (25) extended the simple theory of disloca tions to include the effects of solute atoms on the dislocations. He considered the energy of the solute atom as the strain energy created in the system by the expansion or contraction of the solvent atoms to accommodate the solute atom. If the medium is otherwise stress-free, this strain energy is entirely due to the elastic resistance of the material surrounding the solute atom; but if the strain occurs in a stress field, work will be done against the forces acting on the solute atom from this field. This work alters the total strain energy of the system by an amount termed the energy of interaction between the solute atom and the stress field. The solute atom, consequently, experiences a force 32 drawing it to the region where it can relieve the most stress. Since the interaction energy is large enough to modify the solute distribution near a dislocation, it modifies the dis location behavior. If the solute atoms are larger than the solvent atoms they will be drawn into the tensile part of the dislocation and form an atmosphere of solute atoms at the dislocation. External force exerted on a dislocation tends to move it along a slip plane through its atmosphere which then exerts a counter force on the dislocation. Therefore atmospheres tend to anchor dislocations. If the external force is insufficient to tear the dislocation away from its atmosphere but is suf ficient to produce motion, then the atmosphere will be dragged along with the dislocation; and if the motion reaches constant velocity, then creep occurs; if the external force reaches and exceeds the maximum resistance that the atmosphere can offer, then the dislocation will be torn free from its atmosphere, acceleration of the dislocation takes place and yielding occurs. In a later paper, co-authored with Bilby (26), the statement is made that the yield point of iron is caused by the carbon or nitrogen atmosphere around dislocations. Eshelby (27) observed that damping resulting from thermal fluctuation due to reversed stressing is insufficient to account for actual experimental damping. The dislocations in a metal subjected to vibration oscillate in the stress troughs 33 in the distribution of stresses throughout the crystals. This oscillation of dislocations produces an energy loss and there fore contributes to the damping. If the applied stress is insufficient to lift the dislocations out of the troughs and over the adjoining barriers, the deformation is not permanent and elastic waves are radiated through the metal, said such dislocations are "elastically bound.11 Eshelby In commenting on the observation that damping increases with static stress he presumed the static stress increased the number of disloca tions. In summarizing his ideas on the yield point in single crystals and also polycrystalline metals, Cottrell (28) identified the yield point phenomenon by four characteristics: (a) plastic flow starts at a critical stress (the upper yield point) and can then continue at either the same stress or a lower stress (the lower yield point); (b) a specimen that has yielded (overstrained) shows a smooth transition from the elastic to the plastic range, instead of a yield point, if it is immediately retested; (c) an overstrained specimen recovers the ability to exhibit a yield point if it is rested or annealed; and (d) the preceding effects are observed only if small quantities of certain impurity elements are present in the metal. Cottrell's dislocation theory of the yield point rests on four main ideas as follows: (a) the anchoring of dislocations 34 by solute atoms, (b) the large force needed to release an anchored dislocation, (c) the effect of thermal fluctuations in helping dislocations break away at low stress, and (d) the forced release of anchored dislocations by the pressure of other dislocations previously released. Lomar (29) stated that, in mild polycrystalline steel, local plastic deformation called Lueders1 strain begins at the upper yield point in small regions called Lueders' bands (discovered by Lueders in i860). Once the plastic deformation begins the stress drops to a lower yield point, the extension continues and the Lueders' bands spread, covering an increas ing area of the specimen. When the strain reaches the end of the yield range the bands cover the entire specimen and the extension corresponds to a mean strain equal to the Lueders' strain. When the strain exceeds the yield range the material work-hardens, the stress rises, and the deformation becomes homogeneous throughout the specimen. He termed the permanent strain corresponding to the end of the yield range the Lueders' strain and stated "There appears to be no way of in vestigating the mechanical properties of steel at plastic strains less than the Lueders' strain." This implies that the horizontal yield portion of the stress-strain curve cannot be used to confirm experimentally the theory of an ideal plastic material. Having acknowledged that grain boundaries and impurity 35 atoms act as barriers to dislocation motion he listed the fol lowing factors as governing the lower yield stress and Lueders1 strain: (a) grain size, (b) composition, (c) temperature of specimen during test, (d) heating and strain history, (e) size and shape of specimen, and (f) strain rate. The magnitude of the yield stress increases with decreasing grain size. Single or double (complex) Lueders1 bands may form under strain; the complex bands are associated with higher mean yield stress and a more irregular stress-strain curve—the stress drops with the formation of each new tongue of deformation. Broadly speaking, heavy stiff specimens yield in complex patterns, while lighter flexible specimens yield in single bands. Up to room tempera ture the yield stress varies with the square root of the temperature, while above room temperature aging effects change the behavior of the material. As most other investigators had he, too, found that yield stress rises rapidly with the speed of straining. Lomar found the Lueders1 bands bounded by planes which are near planes of maximum shearing stress. In ten tests the normal to the bounding plane made an angle of 48-1.5° with the tensile direction, which he concluded is a true deviation from the maximum shearing plane at 45° with the tensile direction. At the band front there is a sharp, well defined shear, but in addition there is some other considerable component of extension. He found the shear at the band 36 boundaries in a steel of 40 grains per millimeter accounting for 50 percent of the total extension. The shear "kinks" the bar which induces bending moments to straighten the kink, and the bending influences the band pattern. Barber (3) determined the specific damping capacity for several alloy steels, carbon steels, cast iron, copper, brass, and aluminum by a free torsional oscillation method using a Cambridge Torsional Damping Recorder. He used specific damping capacity as the difference between the maximum potential strain energy at the beginning and end of a cycle divided by the maximum potential energy during the cycle. By restricting his investigation to stresses within the propor tional limit, so that the maximum stresses are proportional to amplitude, he was able to show that the difference in the squares of successive amplitudes divided by the square of the original amplitude gives the specific damping capacity. In general he found much lower damping capacities for alloy steels than for carbon steel, and greater damping capacity for cast iron than steel. Weertman (30) shared the opinion of Nowick (31) that internal friction in single crystals is due to motion of dis locations. They believed the phenomenon of internal friction in cold-worked metals can be divided into three regions or effects. The first effect, characteristic of annealed and slightly cold-worked metals, is due to a hysteresis phenomenon 37 in which dislocations are moved from one low energy position to another, and this effect can be removed by moderate cold working. It also decreases as impurities increase. Nowick said this effect is amplitude dependent while Weertman proposed a dislocation hysteresis model which makes the effect amplitude independent. The second effect, characteristic of moderately cold-worked metal, assumes that dislocations which are loosely bound in the interior of subgrains as a result of cold working move to tighter binding positions at the subgrain boundaries where they cannot contribute much to energy loss. The high internal friction of this effect is unstable and decays rapidly when annealed at low temperatures. The third effect, characteristic of severely cold-worked metal, is due to motion of dislocations in the subgrain boundaries. The motion in creases with temperature which means the internal friction of this effect is temperature and probably frequency dependent. As a consequence of the approximations which Weertman made, the results are valid only if the impurity distribution is random and the dislocations are not pinned down. Of course any interaction between dislocations reduces the number of dislocations with a resulting decrease in internal friction. Granato and Lucke (32) assumed there exists in a pure single crystal, before any deformation due to external con ditions, a network of dislocations. The lengths of the dislocations are determined by the network intersections and 38 are called network loop lengths. For sufficiently large con centrations of impurity atoms these loop lengths are converted into shorter lengths by being pinned down by Cottrell atmos pheres, and these shorter lengths are called impurity loop lengths. When the specimen is subjected to sufficient external stress both elastic strain and dislocation strain occur. At low frequencies, i.e. up to the kilocycle range, the stress-dislocation strain relation is not frequency dependent while at higher frequencies it is frequency de pendent. The dislocation action may be explained with the sketch of Fig. 5 as follows. At A there is no stress applied. As stress is applied the dislocation between impurity atoms bow out as at B and dislocation strain appears. As the stress is increased the loops bow out more as at C and when the stress becomes large enough the dislocation is torn free of the impurity pinning as at D. It is assumed that the ends of the dislocation at the network intersection are so tightly anchored that they do not break free at this stress. In the range up to C the effective modulus of the stress-dislocation strain curve is governed by Lej once the break away occurs, the modulus is governed by Ln. As the stress increases closed dislocation loops form and break away. The dislocation strain past C is plastic but the collapse of the loops on re ducing the stress is elastic. Since there are two moduli involved for straining but only one—dependent on Ln--for 39 U, - Network L oop Lc ~ impurity Loop -o T T 0 Low Stress field Increasing Fig. 5. High Stress Field Stress Progressive dislocation action—from Granato and Liicke (32) 40 collapse of strain, there is a mechanical hysteresis effect. Forscher (33) observed that even though the total stress in a specimen in equilibrium equals the external load, the actual unit stress varies from grain to grain. Slip is a localized action that occurs grainwise with the total stress redistributed to the remaining unslipped grains; the amount of stress redistributed to the neighboring grains depends on the work-hardening capacity of the slipped grains. If the work- hardening capacity is low the stress distribution becomes more heterogeneous finally resulting in catastrophic yielding along surfaces of maximum shear stress. The yielding proceeds by the formation of relaxation centers which are submicroscopically small lens shaped regions of high lattice disorder which, according to Forscher, are quasiviscous, i.e. time and temper ature dependent. Forscher proposed for the density or size of the relaxation centers the expression t - t a £e (<*y " <£) ny T where t is time,(f and a are material constants, and T is the re laxation time from the Arrhenius-type expression T = T0(e)HT - He stated yielding does not depend on a critical stress, but rather on a limiting internal structural condition. This 41 condition, which determines the instant of yielding, is de veloped through stress application. Since each relaxation center introduces a small finite anelastic deformation, n^ implies a limiting amount of anelastic strain. Also since polycrystalline steel consists of ordered crystals separated by disordered quasiviscous regions, Forscher thought of it as a two component system. Chemical composition, temperature, heat-treatment, aging, precipitation, recrystallization, elastic and plastic defor mation, and the state of stress affect in a complicated way the shape, location, proportions, and relative strength of the quasiviscous regions. He assumed no relaxation centers exist in unstressed metal, and that their rate of formation is about proportional to the number present as a consequence of the decrease of available area resisting shear forces. Wessel (34) stated that before yielding or brittle fracture, dislocations move through the lattice, stop, and pile up at barriers which causes appreciable pre-yield plastic strain. This pre-yield plastic strain is maximum at the transition temperature (approximately -196 C for mild steel). Above the transition temperature abrupt yielding occurs when the stress concentrations produced by piled-up dislocations become large enough to overcome resistance to deformation. Sources in adjoining material are activated at this stress level which triggers a general catastrophic yielding. 42 Resistance to plastic deformation below the transition temper ature is so great the dislocation pile-up continues until stress concentrations reach the level that produces microcracks, and set off a sharp catastrophic yielding which ends in brittle failure. Murphy (35) pointed out that microscopic examination of stressed metal reveals definite planes along which slipping or gliding has occurred. This slipping appears to occur along planes of weakness within each crystal, rather than between crystals. The smaller the crystals of a given metal are and the more random their orientation is, the stronger will the metal be. The strength obtained from actual metals is, to a first order of approximation, only about 16 percent of their theoretical strength. This loss in strength is due to imper fections which are termed dislocations. He also observed that the maximum stress in elastic action to which a metal may be subjected can be increased by cold working which causes inter action and dissipation of the dislocations. There are many points in the field of stress-strain relationships of metals upon which different investigators are not in full agreement. However, it appears there is general agreement on the following statements. 1. On a macroscopic scale Hooke's law is valid for most engineering materials over a limited range. 2. Stress is not linearly proportional to strain on a 43 microscale for engineering materials. 3. On a macroscopic scale there is some minimum stress at which gross slipping on planes of weakness, rotation of crystals, and possibly twinning occur. This stress is termed the elastic strength of the material, and is frequently measured by either the proportional limit or the yield strength corresponding to some specified offset. 4. The slipping, rotating, and twinning is frequently incited at low stress levels by imperfections such as dis locations. While a single dislocation is microscopic the total effect in polycrystalline metals is macroscopic. 5. One of the most sensitive measures of the plastic action that has occurred in a material is the change in the damping capacity of that material. 44 ANALYSIS The problem to be solved in this investigation is the prediction of the engineering stress-strain relationship for low-carbon steel in axial tension from the experimentally determined relationship between torsional stress and damping. Much of the work associated with this area of study has been done on a microscopic scale with single metallic crystals. This investigation deals with polycrystalline steel on a macroscopic scale. As the tensile load on a low-carbon steel wire is in creased from zero the metal obeys Hooke's law, and the elongation is proportional to the load up to the proportional limit. This is true on a macroscopic scale, even though individual crystals with unfavorable slip plane orientation may undergo inelastic action before the average or overall stress in the wire reaches the proportional limit. Not only is Hooke's law obeyed by the wire in the proportional range, but the overall action is also essentially elastic which means that relatively little plastic action occurs below the nominal proportional limit in tension. However, as the load is in creased beyond the proportional limit the overall action of the wire departs more and more from Hooke's law which implies that an increasing amount of plastic action has occurred. At any stress level below rupture part of the total strain is elastic and part of it is plastic; i.e. some of the crystals 45 have been permanently deformed while the others are still acting elastically. If the percentages of any transverse area of the wire that are in elastic and plastic action, and if the measure of work-hardening due to plastic action were known, then the nominal or engineering stress-strain relationships could be determined. Therefore, this analysis proceeds in an attempt to determine these facts. One may imagine that the wire is made up of many little bundles of crystals with the bundles axially aligned. It may be postulated that all of the crystals in any given bundle have the same orientation of their slip planes, but that the orientation of slip planes differs from bundle to bundle in a random manner. Plastic action occurs in any given bundle when the shear stress on the slip planes in that bundle reaches and exceeds the elastic limit in shear. Since the shear stress on the slip planes of a bundle is a function of the axial stress in the bundle and the angle between the slip planes and the axial direction, plastic action occurs in the bundle when the axial stress reaches and exceeds the elastic limit of the bundle in axial tension. The effect of slip in one bundle, or even several bundles, on the overall action of the wire is so small that it is not detected in the usual tensile test of steel—this statement can be verified by observing any stressstrain curve in the proportional range for steel. However, when an appreciable number of bundles undergo plastic action, 46 the overall action of the wire, as represented by a tensile stress-strain curve, departs from Hooke's law, and the usual elastic strength in tension is exceeded. Therefore, the over all or average elastic strength of the entire wire may be used to predict the onset of significant plastic action in the wire. It is quite customary to use the proportional limit as a measure of elastic strength. Since the orientation of slip planes from bundle to bundle is random in commercial steels, the likelihood of exceeding the elastic or proportional limit in a bundle at one position in any transverse cross-section of the wire is no less nor no greater than that at any other position in the cross section when the wire is under axial load. If any transverse area of the wire is considered sub divided into many small segments, then each small segment of area may be postulated to be an end of one of the small axially aligned bundles. There will then be a one to one correspondence between the small segments of area and the small bundles of crystals. As load is applied axially to the wire, each bundle undergoes deformation and exerts resistance to the deformation. This resistance, which is the induced unit stress, varies from bundle to bundle in response to the deformation which varies from bundle to bundle. This variation in deformation and stress is the result of the variation in slip plane orientation and imperfections such as dislocations; 47 i.e. for a given unit axial elongation the shear stress on some slip planes is greater than that on other more favorably oriented slip planes. Stated in other words, more axial force is required to produce a given unit elongation in bundles with favorably oriented slip planes than is required to produce the same deformation in bundles with less favorably oriented slip planes. Therefore, the total axial force, F^, acting on the wire is the sum of that part, Fg, acting on the elastic bundles and that part, F^, acting on the plastic bundles which may be written as the equation Ft = Fe + Fp U) • The total transverse area of the wire at any cross section is designated A^., lying in The elastic bundles have end areas which sum to a total elastic area of Ag. Similarly for the plastic bundles, the sum of end areas lying in Aj. sum to Ap. Stated as an equation, ^ = Ae + Ap . (2) The axial stress on the end of any elastic bundle is simply the axial force on that bundle divided by the end area in A^. A similar statement is true for the bundles in plastic action. However, it is impracticable to find the force on each small bundle. Therefore, if the total elastic area in A^ and the sum of all the axial forces acting on the elastic bundles with ends lying in A^ are considered, the relation between them may be 48 written Fe = SeAe (3) where Sg is a composite or average of all the elastic axial stresses acting on A^.. A similar equation relates the com posite plastic axial stress, S , with its plastic area, A , and axial plastic force, Fp. Denoting the quotient of the total axial force, F^., and the total transverse, A*., as the nominal or average engineering axial stress, Sfi, Eq. 1 may be written SA whence = SeAe + SpAp (4) Sn = Sg(^) + Sp(^) . It follows from Eq. 2 that (22) and (5) are the fractions of the total transverse area that are under elastic and plastic action, respectively. It is not unreasonable to assume that the bundles under elastic action obey Hooke's law at any Sg, i.e. Young's modulus, E, is a constant for the portion of the wire under elastic action even if Sg exceeds Sfi at the usual proportional limit. It is postulated that plane transverse areas of the wire remain plane as the axial load increases, so that the unit axial strain, £, is the same for all bundles, both elastic and plastic, that are intercepted by A^. Therefore may be replaced with its equivalent E €. To get an equivalent expression for one might assume an ideal "elastic-plastic" 49 material, i.e. the material obeys Hooke's law up to the elastic limit after which strain increases at constant stress. This gives a horizontal line in the tensile stress-strain curve at a stress magnitude equal to the elastic limit and implies zero work-hardening. Preliminary investigation indicated finite work-hardening did occur in the wire at stresses beyond the usual proportional limit and thus ruled out the assumption. It is therefore assumed that the material obeys Hooke's law up to the elastic limit at which stress the slope of the stressstrain curve changes from Young's modulus, E, to some smaller slope. In this latter assumption, illustrated in Fig. 6, the smaller constant slope implies constant work-hardening, and the slope, B, is the coefficient of work-hardening. The curve in Fig. 6 is for a single bundle of crystals. The stress-strain curve for the entire wire is a composite of the contributions from each bundle. Fig. 7 illustrates the action of several bundles superimposed on each other. stated above, As does not reflect the plastic action of the first few bundles. For a single bundle, it is assumed that plastic action begins at Sy, the proportional limit in shear. However, as previously stated, since the axial and shear stresses are proportional to each other, Sy may also represent the proportional limit in axial stress. It is to be expected that the proportional limit in shear is the same for all the bundles, but the axial proportional limit varies from bundle 5o e Unit Strain Fig. 6. Stress-strain diagram for a single bundle Unit Fig. 7. Strain Stress-strain diagram for a group of bundles 51 to bundle as the slip plane orientation varies. Thus S1 -5 in Fig. 7 represent the axial proportional limits of five different bundles while Sy is the composite axial proportional limit of all five bundles. Referring to Fig. 6, one may write S = S and + AS (6) AS = B( € - € ) (7) where £y is the unit strain corresponding to Sy. Therefore for a single bundle in plastic action Sp = Sy + B( « - €y) and Hp =^= SyAp + B( £ - (8) . (9) Since it is impracticable to measure the axial forces acting on and the transverse area of each bundle, it is assumed that the overall action of the wire may be generalized from the action of a single bundle by using for Sy and £y the composite axial proportional limit and elasticity illustrated in Fig. 7. These are the usual proportional limit and elastic ity determined in a tensile test. Sn = Eq. 5 may then be written as + Sy(?b) + B( - £y) (^). (10) In order to obtain numerical values for nominal unit stress and strain from Eq. 10, the properties E, Sy, and B, as well as the variable fractions of area, must be determined. may be determined from a tensile test of the wire in a E 52 universal testing machine. Sy may be determined from the same test, although a more accurate value was found in the course of determining the area fractions. B can be found after finding the other constants by using experimental values of Sn, 6. , £y,(^), and (^£) in Eq. 10. The literature survey indicates that one of the most sensitive means of detecting plastic action is by measuring the change in the damping capacity of a material. One of the simplest methods of finding the damping capacity of a material is to use the material as a simple torsional pendulum and to measure the decrease of its amplitude in free vibration. As the axial load is increased the plastic action increases and the damping should therefore increase also. This method was selected to determine the damping capacity at a given axial stress level and the change in damping capacity as the axial stress level changes. The stress-damping relationships found in the literature were for torsional stresses in the propor tional range in which the stress was constantly changing during any cycle of vibration. In this investigation, the torsional stress is so small relative to the axial stress that it is neglected when considering plastic action resulting from axial load. The torsional damping is therefore used only as a tool to measure the plastic action resulting from axial stress, which is constant throughout any given cycle of vibration. 53 Specific damping capacity is defined as the ratio between the energy transformed, i.e. the hysteresis, during an oscil lation and the total energy stored in the material by torsion at the beginning of the oscillation. For any differential shell of radius r, thickness dr, and height dy, the energy stored by torsion is ^ T if(27Tr)drdy where T is the torsional unit stress and the wire. if is the torsional unit strain at radius r in If the total angle of twist in the wire pendulum is small, the torsional stresses will be in the proportional range and T = 2f= % 2f where c is the radius of the wire and c m 7 c m the subscript m indicates maximum values which exist at r = c. Therefore, if the energy stored is U, one may write d(U) = ^ T<f(27Tr)drdy = 77Tm ^m~£rr3drdy • (11) For any length of wire whose volume is V Eq. 11 integrates to u"'iT.r»v- (12) If the hysteresis loop is assumed to be parabolic as shown in Fig. 8, the hysteresis, which is the area enclosed in the loop, at any point in the wire is 3 Th, where h is a parameter measuring the distance from the vertex of one loop of the para bolic boundary to the vertex of the other. The difference between h measured normal to the parabolic boundaries or hori zontally as shown is negligible. Assuming h is a function of r so that h = %h_ where hi is the maximum value of the paramc m m eter at the outer surface of the wire one may write for any 54 Unit Torsional Strain, V Fig. 8. Assumed parabolic hysteresis loop A C Fig. 9. Effect of damping on torsional vibration 55 differential shell d(H) = ^Th(277r)drdy = ^Tmhm(J)2(27Tr)drdy (13) where H is hysteresis. For any length of wire whose volume is V, Eq. 13 integrates to H " 3TmhmV ' (14> Therefore the specific damping capacity, D, for the wire is u " For any differential bundle of crystals at any radius r from the axis of the wire 0 =|Vn(e^dV = 4 ik . 5Tm^m<f)2dV 3 (16) ^ Therefore the specific damping capacity of the material is independent of the position in the wire at which the determina tion might be made so long as the torsional stresses are within the proportional range. In this investigation the initial double amplitude and the final double amplitude after ten oscillations were measured. It therefore is necessary to get a measure of the damping in terms of the ten oscillations. Figure 9 represents ten cycles of the decaying free torsional vibration of the wire pendulum, x is approximately equal to 240, where Q is the angular amplitude of twist of the pendulum. At the positions of 56 maximum S , such as A, C, or E, the torsional energy is all potential strain energy while at positions of zero &, e.g. B, D, or F, the energy has changed to kinetic energy. If U is the strain energy at positions of maximum 0 and T is the kinetic energy at zero 9 , the following equations may be written where the subscripts refer to Fig. 9. U A=ï r m r n, V - (17) Tg = UA - hysteresis loss = UA - t;DUa = U^ll - ijD) . (18) UC = TB - 2°TB = TD V1 " l = V1 - l > • = UC " lDUC = D) UA(1 D 2 " 2°)3 • tl9) l2°) At the end of ten oscillations 1 40 UA, = UA(1 - |D) and , (21) Uc, = UA(1 -|d)" . (22) The energy equations in terms of amplitude may be written as follows. 2 ua and Whence and Whence =KX1 = Uc = ~(^)2 = Kx* = Kxfu - -|d)2 . (23) (24) x2 = x1(1 - ^)) , (25) UE = Kx* = Kx,(l - |d)4 . (26) X3 = x1(1 - %D) . (27) 57 2 Similarly, 2 1 4 - 0 UA, = Kx2t = Kxt(1 -|D) 1 20 1 21 X21 = Xi(l - |D) Similarly, Xg2 = x,ll - ^D) , (28) . (29) . (30) The initial double amplitude, as shown in Fig. 9, is a = x, + X2 = x, + x,(l where g is (1 - ^)). -|D) = x,(1 +g) (3D Similarly, the final double amplitude is b = x21 + x22 = x,g 20 + x,g 21 20 = x^g (1 + g) , (32) 20 I= • <33) For ten cycles the specific damping capacity, D', is 2 D' = K*' ' 2 = x 2 ' ' 2 40 = 1. g * ° = 1 - ( f e ) 2 2 2 Kx1 X1 3 2 D' = a 2 " b . 2 a (34) The maximum damping capacity of the steel wire is attained when the maximum plastic action occurs which is just before fracture of the wire. If it is assumed that the plastic action prior to reaching the proportional limit is negligible, a plot of axial stress versus damping capacity should and does show a distinct change at the proportional limit in axial stress. Fig. 10 is a plot of Sfi against D'. If the change in damping at stresses greater than the proportional limit are measured 58 140 1 A Dmcr*. "Z 120 (X too O/ oyo 1 ^ o o p o /bo o OCT )0 I 700 o by Jl o ofo <0 60 oop cP ojp O Co J O 0° 4-0 — d<9 Experimental Calculated 20 — Occp / 1 1 10 Fig. 10. o ao 1 I ; I 1 I JO 4-0 so Axial tensile stress versus damping capacity for ten cycles 59 from the extrapolated curve that holds below the proportional limit to the actual stress-damping curve, then the ratio of the change in damping at any axial stress to the maximum change in damping at fracture represents the increase in plastic action that has occurred. Assuming that all of A^ is plastic at fracture and that approximately none of A^ is plastic below the proportional limit, then the above ratio of changes in damping is equivalent to (A^/A^.), the fraction of the total transverse area that is plastic. The difference between unity and the plastic fraction is the elastic fraction (Ae/A^). One is now in a position to substitute experimental values in Eq. 10 and solve for B, the coefficient of workhardening. B having been found, Eq. 10 can be used to predict the axial stress corresponding to a given axial strain, or the axial strain corresponding to a given axial stress. 60 EXPERIMENTAL PROCEDURE The material tested was No. 18 SAE 1010 steel wire. This wire did not exhibit a yield point when tested in tension on a universal testing machine. The strain was measured with a twostrand SR-4 gage. Figure 11 is a stress-strain curve plotted from data obtained in a tensile test of the wire using a univer sal testing machine and an A-9 SR-4 strain gage. The slope of this curve gives a modulus of elasticity of 28.3(10) psi. The purpose of this tensile test was only to determine the modulus of elasticity, so this specimen was not fractured. Other specimens tested gave an ultimate strength of 132,000 psi. Following the recommendations of several investigators the wire was used as a simple torsional pendulum, usually approximately 20 in. in length, to determine its damping capacity. (See Fig. 12.) One end of the wire was wrapped around a fixed horizontal 2-in. diameter pipe and clamped on the pipe with a small steel bar and C clamps. The other end of the wire was inserted into a holding fixture equipped with hardened set screws. A weight table was rigidly attached to the holding fixture with a 3/8-in. steel rod. A small mirror on the holding fixture reflected a spot of light on a screen 24 in. behind the wire. A lead weight was placed on the table and the pendulum was twisted until the spot of light was 61 120 100 80 <o 20 O / 3 4- e, (/of Fig. 11. Tensile stress-strain diagram for the wire used S 62 rigid pipe frame C damp =0 Jteei damp bar 24- 20 (appro*) wire specimen m/rror 6- 4-4 beotW cte<! / screen iio/ht source zzzza -weight table wet of ht w/re —\ Y"- set screw, 2 reqd. j 4> steel rod ^stocK ^ stee/ rod Holding Fixture Fig. 12. Diagram of apparatus Detail 63 deflected approximately 6 in. from its equilibrium position. The assembly was then released and the maximum travel of the light spot on the opposite side of the equilibrium position was marked. At the tenth oscillation the deflection of the light spot to the left and right of the equilibrium position was again marked. The above procedure was performed on each specimen with the load varying from 8 lb to approximately 200 lb in incre ments of 8 to 11 lb. It is to be noted that the axial tension was constant for each test of ten oscillations. Special care was taken to see that the ends of the wire were firmly gripped, and remained firmly gripped throughout the test. In many of the tests the wire slipped in the grips during the course of the experiment, and since it was not possible to determine exactly when the slipping occurred, the entire results for such tests were discarded. It was also observed that when a nearby turbine was operating the specimen picked up or responded to the turbine vibration. Therefore all tests that were performed during the times at which the turbine was operating were discarded. The results of this investiga tion are based on the tests of five specimens; during these tests nothing appeared to occur which would invalidate the results. follows. A typical set of data recorded on March 24, 1958 64 Table 1. Typical load amplitude data Axial load lb * b+ in a in Stress § psi Damping capacity * 12 3/8 11 7/8 5,500 7.92 17.17 12 15/16 12 5/16 9,800 9.43 25.94 12 j/4 11 15/16 14,660 12.34 42.82 12 9/16 11 13/16 24,100 11.59 51.42 12 1/16 11 3/16 28,800 13.98 59.8'' 12 3/16 11 33,700 18.54 69.82 12 3/16 11 4/16 39,400 14.79 78.41 12 3/16 11 12/16 44,300 15.90 102.03 12 7/16 11 3/16 57,600 19.01 112.20 12 1/16 10 15/16 63,500 17.78 123.30 12 7/16 11 1/8 69,700 19.99 9.73 * a is the initial double amplitude. + b is the double amplitude after 10 oscillations. ®Wire diameter = 0.0475 in; gage length = 20 7/8 in. 65 CALCULATIONS AND RESULTS Nominal or engineering stresses are the average axial stresses obtained by dividing the axial loads by the original transverse area of the wire. The wire tested had a diameter of 0.0475 in. which corresponds to an area of 0.00177 sq in. For a load of 9.95 lb the stress is s n = ^ = o?00177 = 5f,62° psl ' (35) In one of the tests with the load above the initial double amplitude, a, (see Fig. 9) was 11 1/2 in., and the final double amplitude, b, was 10 29/32 in. The damping capacity for this set of values is D* = "2^2) = 0.1006 . (36) It was found during the study of the experimental data that definite trends appear if the axial stresses are plotted against the ratios of axial stress to corresponding damping capacity. Using logarithmic coordinates the trend is a straight line with a positive slope for stresses below the proportional limit, while with semi-logarithmic coordinates and stresses above the proportional limit the trend is a straight line with a negative slope. The point of inter section of the curves representing the two trends is at a stress equal to the proportional limit as obtained from an experimental stress-strain curve. Two equations were selected therefore to represent the 66 two trends. For stresses below the proportional limit the equation is c Sn " m (37) K(tr?> while for stresses above the proportional limit the equation is Sn = kUO) (38) The observed data from five sets of tests are recorded in Table 2. These data reduced to stresses, damping capacities, and stress-damping capacity ratios are presented in Table 3> while these reduced data in logarithmic form are presented in Table 4. The first forty-two sets of data are treated by the method of averaging described by Lipka (.36) to obtain the constants in Eq. 37. In this method the data are divided into two equal or approximately equal groups, and a single equation deduced from each group. This single equation is obtained by adding the equations resulting from substitution of each set of experimental data in the basic equation. The two single equations obtained, one from each group, are then solved simultaneously to obtain the constants. The basic Eq. 37 is first written in logarithmic form to obtain a linear type, Y = C + MX, before Lipka1 s method is applied. g log Sfi = log K + m log (57) (39) 67 Table 2. Observed loads and double amplitudes Run load lb 9.73 A a» a * b t 378 360 a ¥ D b t 382 356 380 360 25.35 392 368 391 369 34.12 378 354 388 364 42.62 386 360 383 358 386 360 375 352 390 362 375 350 390 368 396 372 382 360 382 358 374 353 390 364 386 376 390 361 376 356 374 342 382 358 390 353 390 352 392 366 390 360 76.19 78.41 ¥ 386 358 68.03 69.82 b * 402 378 59.60 59.85 * 408 382 51-00 51.42 a 414 394 17.91 42.82 E b t 368 350 17.39 25.94 a 396 380 9.95 17.17 C B b 392 362 410 376 84.52 386 92.56 386 356 358 334 00.88 388 358 368 342 362 361 337 ^Dimensions expressed in 32nds of an inch 68 Table 2 (Continued) Run load lb 102.03 B A a b ¥ a ¥ C b ¥ a ¥ D b ¥ 384 356 368 338 384 352 362 331 128.28 384 348 357 321 136.62 384 348 352 315 146.59 380 340 358 156.76 380 338 374 324 165.48 378 332 370 318 177.40 374 320 352 296 386 a ¥ b ¥ 350 118.53 123.30 ¥ E b ¥ 398 358 109.47 112.20 a 378 348 398 369 382 342 406 360 380 326 386 344 374 304 388 330 300 400 324 398 356 182.48 188.50 318 372 310 191.20 376 For each group f y f log Sn = f log K + m ^ log (~) (40) Table 3. Run Sn ksi 5-5 Axial stress, corresponding damping capacity, and stress-damping capacity ratio D' A Sn % 7.92 B Sn D» D' D' psi % psi % 60,691 10.06 C » psi D« D D' 5» % psi % E » psi 69,444 9.26 5.6 9.8 D' 55,865 11.41 9.43 103,712 10.1 14.3 8.94 113,087 10.25 85,890 11.75 83,404 98,634 11.87 120,472 10.94 130,713 14.7 12.34 118,801 185,206 10.71 180,205 11.19 172,029 12.17 158,422 19.3 10.41 24.1 11.59 208,001 13.02 185,100 12.63 190,815 28.8 13.98 207,439 13.02 221,198 11.89 242,220 10.91 33.7 18.54 182,308 13.84 243,353 12.89 261,443 38.4 12.83 299,922 39.4 14.79 266,396 43.0 44.3 15.90 278,616 14.72 292,120 12.62 263,978 12.89 223,429 304,279 14.32 268,296 Table 3 (Continued) Run Sn ksi A D' % B Sn D» psi D» % & psi D1 % D' psi & psi D' % 47.8 12.05 396,680 12.85 371,984 10.35 461,386 16.38 52.3 14.94 350,402 12.96 57.0 14.87 57.6 19.09 psi 291,819 403,549 381,977 13.63 418,195 12.17 468,365 18.07 315,440 301,729 61.9 14.05 440,569 15.64 395,780 63.5 17.78 357,143 67.0 15.97 419,223 16.39 408,786 15.24 439,632 14.04 477,208 69.7 19.99 348,674 72.5 17.87 405,708 19.15 378,590 77.2 17.87 432,009 19.92 387,048 19.85 388,413 21.30 82.7 19.94 414,744 21.10 88.5 20.88 423,851 24.95 354,709 93.5 22.86 409,011 26.13 357,826 373,274 29.29 341,414 100.0 26.79 362,441 392,417 26.40 335,227 20.58 430,029 Table 3 (Continued) Run S„ n D' A ksi % B 5 _n D» D« psi % C S„ _n D» psi 103.0 106.5 108.0 D» % D S„ n D" psi D' % 33.93 30.56 E S„ __n D» psi D« % 303,566 27.66 S„ _jn D' psi 373,188 348,495 36.34 297,193 34.39 314,045 72 Table 4. Axial stress and logarithms of stress-damping ratios Run A B sn D c sn iog QT 1*9 5? 4.7831 4.7471 sn l°g S„ log or 5,500 3.7404 4.8417 5,620 3.7497 9,800 3.9912 10,110 4.0047 5.0535 4.9940 14,300 4.1553 5.0808 5.1162 14,660 4.1655 19,280 4.2851 5.2677 5.2558 24,100 4.3820 5.3198 5.2674 5.2806 28,800 4.4594 5.3169 5.3448 5.3824 33,700 4.5276 5.2608 5.3861 5.4173 38,400 4.5843 39,400 4.5955 43,000 4.6335 44,300 4.6464 47,800 4.6794 5.5985 5.5705 52,300 4.7185 5.5446 5.6058 57,000 4.7559 5.5820 5.6214 57,600 4.7604 61,900 4.7917 5.6440 5.5975 63,500 4.8028 Sn E Sn Sn DT 109 D? lo 9 4.9340 4.9212 5.2356 5.1998 5.4216 5.3491 5.4833 5.4286 5.6640 5.4651 5.6705 5.4988 psi 5.0157 5.0749 5.4770 5.4256 5.5655 5.4449 5.4796 5.5528 73 Table 4 (Continued) Run A iog Sn Sn C B E log D? Sn log s? log D? Sn log qt 5.6224 5.6116 5.6431 5.6787 5.5893 5.5592 5.5253 5.6335 5.4822 5.5719 5.4731 5.4969 sn log s? D s n sn psi 67,000 4.8261 69,700 4.8432 72,500 4.8603 5.6083 5.5782 77,200 4.8876 5.6355 5.5877 82,700 4.9175 5.6177 5.5937 88,500 4.9469 5.6271 5.5499 93,500 4.9708 5.6117 5.5537 100,000 5.0000 5.5720 5.5333 103,000 5.0128 106,500 5.0274 108,000 5.0334 5.5425 5.5422 From Table 4, 21 Yi 21 l09 Sn = 87.3635 , Y- c - Or 1o9(dt) = 107.4330 1 42 Y~ 22 42 log s n = 9 7 . 3 0 8 1 , s 21109(57) = 1 1 5 . 4 8 2 0 . 22 If the above values are substituted in Eq. 40 there results 87.3635 = 21 log K + 107.4330 , (41) 74 and 97.3081 = 21 log K + 115.4820 . (42) Simultaneous solution of Eqs. 41 and 42 yields m = 1.2355» log K = -2.I605, and K = 0.006912. Therefore, Eqs. 37 and 39 become Sn = 0.006912(^7) and , log Sn =. -2.1605 + 1.2355 log(§?) . (37a) (39a) The constants in Eq. 38 are obtained by the above method also by using the last twenty-two sets of experimental data. Data in the vicinity of the proportional limit are not used in obtaining the constants for either Eq. 37 or 38 because the scatter in this neighborhood is much greater than elsewhere. Expressing Eq. 38 in logarithmic form log Sn = log k + n(Sû) . (43) If the last twenty-two sets of experimental data in Tables 3 and 4 are used there is obtained: 11 11 log Sn = 53.8430 , S Y- (D?) = 4,288,604 1 1 22 22 y log S 12 = 54.9552 , g y (g?) = 3,883,268 . 12 When these values are substituted in Eq. 43 there is obtained and 53.8430 = 11 log k + 4,288,604 n , 144) 54.9552 = 11 log k + 3,883,268 n , (45) 75 —£ whence n = -2.7439(10) , log k = 5.9646, and k = 921,750 psi. Therefore, Eqs. 38 and 43 become Sn = 921,750(10) 2*7439(10) and log (Dr) (38a) = 5.9646 - 2.7439(10) 6(5?) (43a) Equations 37a and 38a, or 39a and 43a, represent the experimental data quite well as is seen in Figs. 13 and 14. The stress-strain diagram, Fig. 11, was constructed to obtain Young's modulus. Other tests resulted in smooth curves similar to Fig. 11 with rupture occurring at 132,000 psi. It is at the rupture stress that complete plastic action is assumed to occur. However, since it was not possible to measure damping at rupture, the stress-damping curve, Fig. 10, was extrapolated to rupture by evaluating the damping capacity at various stress levels in the plastic range from Eq. 43a. Equation 39a was used to obtain values of damping capacity for extrapolating the proportional range relationship beyond the proportional limit. As noted in the analysis, the difference in damping capacity between these two relationships at rupture is postulated to be the maximum change in damping and to be directly proportional to the maximum change in plastic action. The difference at any lower stress is postulated to be proportional to the change in plastic action at the lower stress. Confidence is 76 placed in the extrapolations because Eqs. 39a and 43a are linear and represent the reduced experimental data quite well. Since the changes in damping capacity are proportional to changes in plastic action the ratio of the change in damping capacity at some lower stress to the maximum change at rupture is the fraction of the material that has changed from the initial elastic state to the plastic condition. At 132,000 psi there is obtained from Eq. 43a c§»> =(5-96t^ Sn)io6 = (?-?6^7;3^206)io6 = 307,591 , whence Dmax = (43b) " °-4291 • At the same stress, 132,000 psi, there is obtained from Eq. 39a log (&) = whence l0? Î1+i5ï1605 = ?-12^ ^f-16°? 2 , (39b) D' = 0.1688 ; therefore, (4D1) = D' v - D' = 0.4291 - 0.1688 = 0.2603 . (46) iuoX lUdX Similarly, at 70,000 psi, AD' = 0.0220 . (47) Tables 5 and 6 present the data used in plotting the stressdamping relationship shown in Fig. 10. «^Dmax and AD' in that figure are the values determined by Eqs. 46 and 47. As is postulated in the Analysis the fraction of the 77 material that has passed from the elastic to the plastic range at 70,000 psi is (A^> = "S5^x = §ti§§ » 0-0845 = 8.45% . 148) The fraction that has not changed from the elastic to the plastic condition is (^) = 1 - (^) = 0.9155 = 91.55# . 149) If the wire is completely elastic before application of the axial load, then (É&) is the total fraction of the material &t that is plastic at Lhe given stress level. However, if the material has been cold-worked prior to the damping test, then Ap (y££) represents the fractional increase of material in the plastic range. In either event, the stress-strain curve that is obtained is the customary tensile test curve that is pre dicted by Eq. 10. The intersection of the curves obtained by plotting Eqs. 39a and 43a in Figs. 13 or 14 is a more easily and more accurately read proportional limit than is the point of tangency at which linearity ceases in a stress-strain curve. The proportional limit in axial stress, 62,500 psi, may be read from either Fig. 13 or 14. It has been remarked earlier that scatter of the stressdamping data is greater near the proportional limit than elsewhere. Plastic action is masked more by the greater amount 78 aoo / — 3 8cr — too 80 o — 60 o 08/T^ 8 <d/t£> \ 40 cp^oo 0 \ ZO £<%- 37ot 10 8 6 / / — / / / -i i ; / 1 100 ZOO 300 (M 40 0 SOO m 13- Axial stress versus axial stress-damping capacity ratio 79 ZO ZO' ZO ZO Fig. 14. zo Axial stress versus axial stress-damping capacity ratio 80 Table 5. ^n psi Values of damping capacity determined from Eq. 3a log Sn log D' (57) psi 1 0 1.7487 56.07 0.0178 5,000 3.6990 4.7426 55,288 0.0904 10,000 4.0000 4.9862 96,875 0.1032 20,000 4.3010 5.2298 169,750 0.1178 30,000 4.4771 5.3724 235,700 0.1273 40,000 4.6021 5.4736 297,600 0.1344 50,000 4.6990 5.5520 356,500 0.1403 60,000 4.7782 5.6161 413,100 0.1452 70,000 4.8451 5.6703 468,000 0.1496 80,000 4.9031 5.7172 521,400 0.1534 90,000 573,600 0.1569 100,000 624,600 0.1601 110,000 674,700 0.1630 120,000 724,000 0.1657 130,000 772,300 0.1683 132,000 782,000 0.1688 140,000 820,200 0.1707 of elastic action near the proportional limit than by the smaller amount of elastic action near the rupture stress. Therefore, the coefficient of work-hardening, B, is determined from Eq. 10 at an axial stress of 130,000 psi which is near 81 Table 6. Values of damping capacity determined from Eq. 7a Sn> log Sn Psi D» (§r), psi 60,000 4.7782 432,377 0.1388 70,000 4.8451 407,996 0.1716 80,000 4.9031 386,858 0.2068 90,000 4.9542 368,235 0.2444 100,000 5.0000 351,543 0.2845 110,000 5.0414 336,455 0.3269 120,000 5.0792 322,679 0.3719 130,000 5.1139 310,033 0.4193 132,000 5.1206 307,591 0.4291 140,000 5.1461 298,298 0.4693 rupture. Solving Eq. 10 for B one obtains A .• A in which H is (-%—) and H is (-r&). Upon substituting values At e Ap P previously determined from the experimental data in Eq. 10a, one obtains B = 130.000 - (28.3)(6.4)(35.7) - 62.500(0.9641) (6.40 - 2.208)(10"3)(0.9643) = 15.65(10)* psi. Values of B determined at various stress levels are given in Table 7. The value found above produces closer agreement with 82 Table 7. Values of B evaluated at various stress levels H,,(10) Hp(10) BUO)6 psi psi E(10)6 psi 130,000 28.3 6.40 2.208 62,500 0.357 9.643 15.65 120,000 28.3 5.25 2.208 62,500 2.078 7.922 16.44 110,000 28.3 4.45 2.208 62,500 3.703 6.297 17.00 100,000 28.3 3.88 2.208 62,500 16.02 Sn €(10)" 3 psi 5.221 4.779 the experimental stress-strain curve than do the values at other stress levels. Equation 10 can be used to predict axial stress from axial strain only if He and Hp have been determined as Table 8. Plastic and elastic fractions at various axial stresses Sn D* Hp"O) H*(10) psi 70,000 0.0220 0.845 9.155 80,000 0.0534 2.051 7.949 90,000 0.0875 3.362 6.638 100,000 0.1244 4.779 5.221 110,000 0.1639 6.297 3.703 120,000 0.2062 7.922 2.078 130,000 0.2510 9.643 0.357 83 Table 9. Stress-strain points determined from Eq. 10c Sn, psi 27,945Hp 28.3He(10)6 15.65% (10)* (10) 70,000 2,361 25.908 1.322 2.48 80,000 5,732 22.496 3.210 2.89 90,000 9,395 18.785 5.261 3.35 100,000 13,355 14.775 7.479 3.89 110,000 17,597 10.479 9.855 4.54 120,000 22,138 5.881 12.398 5.35 130,000 26,947 1.010 15.091 6.40 functions of strain. In this investigation these fractions, recorded in Table 8, have been found as functions of stress only. With this information only strain at a specified stress can be predicted. Therefore, the equation to predict the axial strains corresponding to given axial stresses in the wire is e. . e p Upon substituting the constants previously determined the equation becomes Sn - 27,94% ^ " (2ti.3He + 15.65Hp)10b • (10c) The axial unit strain predicted for an axial unit stress of 70,000 psi is f = 28.3»%^» U0>J = 2.45(10-', . 84 The values for plotting the predicted stress-strain curve of the wire, Fig. 15, are given in Table 9. It is to be noted that for stresses less than the propor tional limit, Sy, in which range plastic action is assumed to be negligible, the prediction equation simplifies to Hooke's law. 85 100 «0 ÔO 60 O Ex/o erimen ta/ Eq. /Oc 20 0 2 6 8 —3 € , 10 Fig. 15. Comparison of experimental with predicted tensile stress-strain diagram 86 CONCLUSIONS The results obtained in this investigation lead to the following conclusions. 1. Plastic deformation in low-carbon steel is a progres sive action. At any engineering or nominal stress level between the proportional limit and rupture a certain finite fraction of the material is plastic and the remainder is elastic. 2. The effect of plastic action on the stress-strain relationship for polycrystalline steel below the proportional limit is negligibly small. 3. The change in damping due to plastic action below the proportional limit is negligible in comparison to the change in damping due to plastic action above the proportional limit. Above the proportional limit the change in damping capacity due to plastic action may be taken as the difference between the extrapolated stress-damping curve that holds below the proportional limit and the stress-damping curve that holds above the proportional limit. 4. On the basis of the agreement of the predicted and experimentally determined tensile stress-strain curves the following postulate appears reasonable: the fraction of any transverse area of the wire that changes from elastic to plastic action as the axial tension is raised to any engineer 87 ing stress level can be expressed as the ratio between the change in damping capacity that occurs in reaching that stress and the maximum change in damping capacity that occurs in reaching the ultimate stress. 5. It appears that the proportional limit may be deter mined by finding the intersection of the curves of stress versus the ratio of stress to damping capacity that hold below and above the proportional limit. This intersection is clearly defined with either logarithmic or semi-logarithmic coordinates. 6. The relationship between axial stress and strain for low-carbon steel wire can be predicted from stress-damping data if the work-hardening coefficient is available. prediction equation as developed herein is g • Sn - BV (SY' EHe + BHp HP . The 88 RECOMMENDATIONS FOR FUTURE WORK It is recommended that this method be applied to metals other than low-carbon steel in order to determine its general applicability. Further study of the work-hardening coefficient, B, is also recommended. It may be observed from Table 6 that B 6 appears to increase with stress to 17(10) psi, and thereafter 6 to decrease to 15*65(10) psi. This may indicate a stress region in which B is variable, or it may result from the masking of plastic action by elastic action. In future work an attempt to improve the wire holding device should be made to prevent slipping at high loads. 89 SYMBOLS EMPLOYED e = area in elastic action Ap = area in plastic action A^ = original transverse area B = work-hardening coefficient D = damping capacity = - E = Young's modulus 2 = elastic component of total axial stress Fp = plastic component of total axial stress F t = total axial stress A H e = = elastic fraction At A H = -7e = plastic fraction p At S = unit stress S = elastic stress e S n = nominal engineering stress S„ = plastic stress P Sy = proportional limit a = initial double amplitude b = double amplitude at the tenth oscillation 90 6 = unit strain = elasticity k, K, m, n = arbitrary constants 91 LITERATURE CITED 1. Doan, G. E. and Mahla, E. M. The principles of physical metallurgy. 2nd ed. New York, N. Y., McGraw-Hill Book Co., Inc. 194-1. 2. Thompson, F. C. Damping capacity. London, British NonFerrous Metals Research Association. 1944. 3-4. Barber, W. J. Determination of the damping capacity of typical metals by a free vibration method. University of Kentucky Engineering Experiment Station Bulletin No. 27. 1953. 5. Lord Kelvin (Sir William Thompson). Mathematical and physical papers. Vol. 1. London, C. J. Clay and Sons. 1890. 6. Joffe, Abram F. The physics of crystals. New York, N. Y., McGraw-Hill Book Co., Inc. 1928. 7. Becker, E. and Fôppl, 0. Dauerversuche zur Bestimmung der Festigkeitseigenschaften Beziehungen zwischen Baustoffdampfung und Verformungsgeschwindigkeit. Forschungsarbeiten auf dem Gebiete des Ingenieurwesens Herausgegeben vom verein Deutscher Ingenieure Heft 304: 1-28. 1928. 8. Templin, R. L. The determination and significance of the proportional limit in the testing of metals. Pro ceedings of the American Society for Testing Materials 29: 523-553. 1929. 9. Moore, H. F. Discussion. Proceedings of the American Society for Testing Materials 29: 535. 1929. 10. McVetty, P. G. Discussion. Proceedings of the American Society for Testing Materials 29: 549. 1929. 11. Withey, M. 0. Discussion. Proceedings of the American Society for Testing Materials 29: 551. 1929. 12. Tuckerman, L. B. Discussion. Proceedings of the American Society for Testing Materials 29: 538. 1929. 92 13. 14. Brophy, G. R. Damping capacity of steels and correlation with other properties. The Iron Age 130: 800-802, 989. 1932. . Damping capacity a factor in fatigue. Transactions of the American Society for Metals 24: 154-185. 1936. 15. Foppl, 0. The practical importance of the damping capacity of metals, especially steel. Journal of the Iron and Steel Institute 134, No. 2: 393P-455P. 1936. 16. Nadai, A. Plastic behavior of metals in the strainhardening range. I. Journal of Applied Physics 8: 205-213. 1937. 17. Spath, Wilhelm. Dampfung und Festigkeitswerte der Workstoffe. Archiv fur das Eisenhuttenwesen 11: 503-508. 1938. 18. Winlock, Joseph and Leiter, Ralph W. E. Some observations on the yield point of low-carbon steel. Transactions of the American Society of Mechanical Engineers 61: 581-587. 1939. 19. Contractor, G. P. and Thompson, F. C. The damping capacity of steel and its measurement. Journal of the Iron and Steel Institute 141: 157P-201P. 1940. 20a. Hatfield, W. H., Stanfield, G. and Rotherham, L. The damping capacity of engineering materials. Trans actions of the North East Coast Institution of Engineers and Ship Builders 58: 274-332. 1942. 20b. Low, John R., Jr., and Garofalo, Frank. Precision deter mination of stress-strain curves in the plastic range. Proceedings of the Society for Experimental Stress Analysis 4, Mo. 2: 16-24. 1947. 21. Zener, Clarence. Elasticity and anelasticity of metals. Chicago, 111., The University of Chicago Press. 1948. 22. Hanstock, R. F. Damping capacity. 383-385. 1948. Metal Industry 73: 23. Cuff, Frank B,, Jr.. and Schetky, L. McD. Scientific American 193: 0O- 8 7 . July, 1955. 93 24. Woolley, R. L. Work-hardening in polycrystalline pure metals. In Report of a Conference on Strength of Solids, University of Bristol, July 7-9, 1947. Pp. 51-56. London, The Physical Society. 1948. 25. Cottrell, A. H. Effect of solute atoms on the behavior of dislocations. In Report of a Conference on Strength of Solids, University of Bristol, July 7-9, 1947. Pp. 30-38. The Physical Society. 1948. 26. and Bilby, B. A. Dislocation theory of yielding and strain ageing of iron. Proceedings of the Physical Society 62, A: 49-62. 1949. 27. Eshelby, J. D. Dislocations as a cause of mechanical damping in metals. Proceedings of the Royal Society of London 197, A: 396-416. 1949. 28. Cottrell, A. H. The yield point in single crystal and polycrystalline metals. In Symposium on the Plastic Deformation of Crystalline Solids, Mellon Institute, May 19-20, 1950» Pp. 60-73. Pittsburgh, Pa., Carnegie Institute of Technology and Department of the Navy Office of Naval Research. 1950. 29. Lomar, W. M. The yield phenomenon in polycrystalline mild steel. Journal of the Mechanics and Physics of Solids Is 64-72. 1952. 30. Weertman, Johannes. Internal friction of metal single crystals. Journal of Applied Physics 26: 202-210. 1955. 31. Nowick, A. S. Internal friction and dynamic modulus of cold-worked metals. Journal of Applied Physics 25: 1129-1134. 1954. 32. Granato, A. and Lucke, K. Theory of mechanical damping due to dislocations. Journal of Applied Physics 27: 583-593. 1956. 33. Forscher, F. Theory of the yield point and the transition temperature of mild steel. Journal of Applied Mechanics 23: 219-224. 1956. 34. Wessel, E. T. Abrupt yielding and the ductile-to-brittle transition in body-centered cubic metals. Journal of Metals 9: 930-935. 1957. 94 35. Murphy, Glenn. Properties of engineering materials. 3rd ed. Scranton, Pa., International Textbook Co. 1957. 36. Lipka, Joseph. Graphical and mechanical computation. New York, N. Y., John Wiley and Sons. 1918. 95 ACKNOWLEDGMENTS The author expresses appreciation to his graduate com mittee for their help and understanding. He is particularly appreciative of the counsel, inspiration, encouragement, and patient understanding received from his major professor and committee chairman, Dr. Glenn Murphy. The author will be grateful always for the cheerful acceptance by his wife and children of the way of life neces sary for her husband and their father to pursue graduate study.